#------------------------------------------------------------------------------
#$Date: 2019-11-23 12:03:07 +0200 (Sat, 23 Nov 2019) $
#$Revision: 233208 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/56/7235660.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7235660
loop_
_publ_author_name
'Saini, Mukesh Kumar'
'Gupta, Rakesh'
'Parbhakar, Swati'
'Kumar Mishra, Anil'
'Mathur, Rashi'
'Hussain, Firasat'
_publ_section_title
;
 Dimeric complexes of rare-earth substituted Keggin-type silicotungstates:
 syntheses, crystal structure and solid state properties
;
_journal_issue                   48
_journal_name_full               'RSC Adv.'
_journal_page_first              25357
_journal_paper_doi               10.1039/C4RA02751E
_journal_volume                  4
_journal_year                    2014
_chemical_formula_moiety         '0.5(C8 Gd4 K16 Na8 O208 Si4 W44), 6(O)'
_chemical_formula_sum            'C4 Gd2 K8 Na4 O110 Si2 W22'
_chemical_formula_weight         6627.92
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_Int_Tables_number      14
_audit_creation_date             2014-03-26
_audit_creation_method
;
Olex2 1.2
(compiled 2014.03.20 svn.r2914 for OlexSys, GUI svn.r4813)
;
_cell_angle_alpha                90
_cell_angle_beta                 110.470(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   20.0905(6)
_cell_length_b                   12.6729(3)
_cell_length_c                   21.0974(6)
_cell_measurement_reflns_used    21143
_cell_measurement_temperature    150.0
_cell_measurement_theta_max      29.1168
_cell_measurement_theta_min      2.8918
_cell_volume                     5032.3(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_diffrn_ambient_temperature      150.0
_diffrn_detector_area_resol_mean 15.9853
_diffrn_measured_fraction_theta_full 0.9986
_diffrn_measured_fraction_theta_max 0.9986
_diffrn_measurement_device_type  'Xcalibur, Sapphire3'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      0.0360923000
_diffrn_orient_matrix_UB_12      0.0161069000
_diffrn_orient_matrix_UB_13      0.0115673000
_diffrn_orient_matrix_UB_21      0.0021650000
_diffrn_orient_matrix_UB_22      -0.0133493000
_diffrn_orient_matrix_UB_23      -0.0318555000
_diffrn_orient_matrix_UB_31      -0.0105938000
_diffrn_orient_matrix_UB_32      0.0519524000
_diffrn_orient_matrix_UB_33      -0.0117670000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0720
_diffrn_reflns_av_unetI/netI     0.0568
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            77033
_diffrn_reflns_theta_full        26.0217
_diffrn_reflns_theta_max         26.02
_diffrn_reflns_theta_min         2.90
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    26.821
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.18286
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    4.3739
_exptl_crystal_F_000             5752.0738
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.04
_refine_diff_density_max         16.0401
_refine_diff_density_min         -3.5228
_refine_diff_density_rms         0.6661
_refine_ls_d_res_high            0.8100
_refine_ls_d_res_low             7.0297
_refine_ls_goodness_of_fit_ref   1.0369
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     389
_refine_ls_number_reflns         9899
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.0369
_refine_ls_R_factor_all          0.0593
_refine_ls_R_factor_gt           0.0520
_refine_ls_shift/su_max          0.0298
_refine_ls_shift/su_mean         0.0004
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0360P)²+547.4914P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1160
_refine_ls_wR_factor_ref         0.1202
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              23
_reflns_limit_h_min              -24
_reflns_limit_k_max              15
_reflns_limit_k_min              0
_reflns_limit_l_max              26
_reflns_limit_l_min              0
_reflns_number_gt                8886
_reflns_number_total             9899
_reflns_threshold_expression     I>=2u(I)
_cod_data_source_file            c4ra02751e2.cif
_cod_data_source_block           FHMS-27
_cod_database_code               7235660
_chemical_oxdiff_usercomment     '12 NOV 2013'
_reflns_odcompleteness_completeness 99.81
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
;
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y+1/2,-z+1/2
3 -x,-y,-z
4 x,-y-1/2,z-1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
C1 C -0.1357(11) 1.0820(16) 0.0715(10) 0.022(4) Uiso 1.000000
C2 C -0.0767(9) 1.0104(13) 0.0671(8) 0.009(3) Uiso 1.000000
O1 O 0.4952(7) 0.8697(10) 0.4332(6) 0.017(3) Uiso 1.000000
O2 O 0.4240(7) 0.5751(10) 0.2242(7) 0.019(3) Uiso 1.000000
O3 O 0.2918(7) 0.5639(11) 0.4094(7) 0.021(3) Uiso 1.000000
O4 O 0.4419(7) 0.7509(11) 0.3166(7) 0.022(3) Uiso 1.000000
O5 O 0.3477(7) 0.5972(10) 0.3092(7) 0.019(3) Uiso 1.000000
O6 O 0.3763(7) 0.7380(10) 0.4093(6) 0.017(3) Uiso 1.000000
O7 O 0.4197(6) 0.9539(9) 0.3049(6) 0.009(2) Uiso 1.000000
O8 O 0.3847(6) 0.7893(9) 0.1883(6) 0.011(2) Uiso 1.000000
O9 O 0.2856(7) 0.6468(10) 0.1789(6) 0.014(3) Uiso 1.000000
O10 O 0.2082(6) 0.6350(9) 0.2831(6) 0.011(2) Uiso 1.000000
O11 O 0.2382(7) 0.7716(10) 0.3817(6) 0.015(3) Uiso 1.000000
O12 O 0.3530(7) 0.9447(10) 0.3929(6) 0.015(3) Uiso 1.000000
O13 O 0.3085(6) 0.7936(9) 0.2850(5) 0.006(2) Uiso 1.000000
O14 O 0.1180(7) 0.8421(10) 0.4081(6) 0.015(3) Uiso 1.000000
O15 O 0.2312(7) 0.9733(10) 0.4102(6) 0.014(3) Uiso 1.000000
O16 O 0.3242(7) 1.1455(10) 0.4379(6) 0.017(3) Uiso 1.000000
O17 O 0.3287(6) 1.1004(9) 0.3072(6) 0.012(3) Uiso 1.000000
O18 O 0.4451(7) 1.1627(10) 0.2733(6) 0.016(3) Uiso 1.000000
O19 O 0.4031(6) 0.9951(9) 0.1782(6) 0.012(2) Uiso 1.000000
O20 O 0.3804(7) 0.8672(10) 0.0653(6) 0.013(3) Uiso 1.000000
O21 O 0.2598(6) 0.7988(9) 0.0905(6) 0.012(2) Uiso 1.000000
O22 O 0.2045(7) 0.5989(9) 0.0466(6) 0.013(3) Uiso 1.000000
O23 O 0.1458(6) 0.6092(9) 0.1471(5) 0.007(2) Uiso 1.000000
O24 O 0.0657(7) 0.5787(10) 0.2291(6) 0.013(3) Uiso 1.000000
O25 O 0.1168(6) 0.7830(9) 0.2824(6) 0.009(2) Uiso 1.000000
O26 O 0.2155(6) 0.9423(8) 0.2830(5) 0.006(2) Uiso 1.000000
O27 O 0.2832(6) 0.9496(8) 0.1956(5) 0.005(2) Uiso 1.000000
O28 O 0.1856(6) 0.7976(9) 0.1843(5) 0.006(2) Uiso 1.000000
O29 O 0.1031(6) 0.9885(9) 0.3091(6) 0.009(2) Uiso 1.000000
O30 O 0.2043(6) 1.1340(9) 0.3229(6) 0.011(2) Uiso 1.000000
O31 O 0.3101(6) 1.1439(9) 0.1776(6) 0.009(2) Uiso 1.000000
O32 O 0.2789(6) 1.0074(9) 0.0776(6) 0.010(2) Uiso 1.000000
O33 O 0.1153(6) 0.7577(9) 0.0485(6) 0.011(2) Uiso 1.000000
O34 O 0.0433(6) 0.7530(9) 0.1488(6) 0.009(2) Uiso 1.000000
O35 O 0.1478(7) 0.9844(9) 0.0870(6) 0.012(3) Uiso 1.000000
O36 O 0.0767(6) 0.9823(9) 0.1758(6) 0.010(2) Uiso 1.000000
O37 O 0.1842(6) 1.1172(9) 0.1910(6) 0.010(2) Uiso 1.000000
O38 O 0.0678(6) 1.1775(9) 0.2301(6) 0.012(2) Uiso 1.000000
O39 O 0.1878(6) 1.1805(9) 0.0619(6) 0.011(2) Uiso 1.000000
O40 O 0.0347(6) 0.9564(9) -0.0380(6) 0.008(2) Uiso 1.000000
O41 O -0.0432(7) 0.7787(10) -0.0042(6) 0.014(3) Uiso 1.000000
O42 O -0.0692(7) 0.9200(10) 0.0927(6) 0.014(3) Uiso 1.000000
O43 O -0.1743(9) 0.8969(13) 0.1826(8) 0.033(4) Uiso 1.000000
O44 O 0.4582(10) 0.9023(15) 0.5871(9) 0.046(5) Uiso 1.000000
O45 O 0.3924(10) 0.3843(14) 0.3203(9) 0.041(4) Uiso 1.000000
O46 O 0.0784(8) 1.3744(12) -0.0978(8) 0.030(3) Uiso 1.000000
O47 O 0.4678(13) 1.2914(19) 0.4440(12) 0.071(6) Uiso 1.000000
O48 O 0.3149(7) 1.3769(11) 0.4830(7) 0.020(3) Uiso 1.000000
O49 O 0.4716(8) 1.4050(12) 0.5931(8) 0.030(3) Uiso 1.000000
O50 O 0.3661(9) 1.1990(14) 0.6112(9) 0.040(4) Uiso 1.000000
O51 O 0.2302(8) 0.3861(11) 0.0324(7) 0.025(3) Uiso 1.000000
O52 O 0.1628(10) 0.3984(14) 0.1308(9) 0.044(4) Uiso 1.000000
O53 O -0.0307(9) 0.6907(12) -0.1180(8) 0.033(4) Uiso 1.000000
O54 O 0.2565(7) 1.3139(11) 0.2495(7) 0.022(3) Uiso 1.000000
O55 O 0.0538(6) 0.9562(8) 0.4802(5) 0.002(2) Uiso 1.000000
Na1 Na 0.4541(6) 0.9445(8) -0.0114(5) 0.041(2) Uiso 1.000000
Na2 Na 0.4058(5) 1.2560(7) 0.5203(5) 0.035(2) Uiso 1.000000
Si1 Si 0.2472(2) 0.8695(4) 0.2357(2) 0.0077(9) Uani 1.000000
K1 K -0.0276(2) 0.8814(3) 0.2317(2) 0.0152(8) Uani 1.000000
K2 K 0.3263(2) 0.8380(4) 0.5089(2) 0.0219(9) Uani 1.000000
K3 K 0.4714(2) 0.3669(3) 0.2380(2) 0.0226(9) Uani 1.000000
K4 K 0.1891(3) 1.2375(4) -0.0690(3) 0.0338(11) Uani 1.000000
Gd1 Gd 0.04573(4) 0.88815(6) 0.07366(4) 0.00750(17) Uani 1.000000
W1 W 0.41438(4) 0.84817(5) 0.36998(4) 0.01169(15) Uani 1.000000
W2 W 0.37162(4) 0.67006(6) 0.24074(4) 0.01201(15) Uani 1.000000
W3 W 0.28945(4) 0.66275(6) 0.35376(4) 0.01209(16) Uani 1.000000
W4 W 0.16255(4) 0.87309(5) 0.35494(3) 0.00883(15) Uani 1.000000
W5 W 0.28529(4) 1.05998(5) 0.37115(3) 0.00947(15) Uani 1.000000
W6 W 0.37768(4) 1.07151(5) 0.24715(3) 0.00809(14) Uani 1.000000
W7 W 0.33888(4) 0.89240(5) 0.12209(3) 0.00814(14) Uani 1.000000
W8 W 0.19422(4) 0.69582(5) 0.10053(3) 0.00791(14) Uani 1.000000
W9 W 0.11270(4) 0.68096(5) 0.21133(3) 0.00786(14) Uani 1.000000
W10 W 0.21669(4) 1.07688(5) 0.11824(3) 0.00764(14) Uani 1.000000
W11 W 0.12560(4) 1.07145(5) 0.23974(3) 0.00803(14) Uani 1.000000
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
C 0.00347 0.00161 2.31000 1.02000 1.58860 0.86500 20.84390 10.20750 0.56870
51.65120 0.215599998832
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Na 0.03665 0.02467 4.76260 3.17360 1.26740 1.11280 3.28500 8.84220 0.31360
129.42400 0.675999999046
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
K 0.21174 0.26561 8.21860 7.43980 1.05190 0.86590 12.79490 0.77480 213.18700
41.68410 1.42279994488
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Si 0.08192 0.07060 6.29150 3.03530 1.98910 1.54100 2.43860 32.33370 0.67850
81.69370 1.14069998264
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Gd 0.10424 4.27310 25.07090 19.07980 13.85180 3.54545 2.25341 0.18195 12.93310
101.39800 2.41960000992
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
W -0.66836 6.76498 29.08180 15.43000 14.43270 5.11982 1.72029 9.22590 0.32170
57.05600 9.88749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O40 C2 C1 119.6(15) 3_575 .
O42 C2 C1 119.9(15) . .
O42 C2 O40 120.5(15) . 3_575
Gd1 C2 C1 172.9(12) . .
Gd1 C2 O40 60.0(8) . 3_575
Gd1 C2 O42 60.8(9) . .
W1 O1 Na2 128.0(7) . 3_676
W2 O2 K3 148.9(7) . .
W1 O4 K3 104.9(6) . 2_655
W2 O4 K3 107.7(5) . 2_655
W2 O4 W1 122.7(7) . .
W3 O5 W2 121.1(7) . .
W1 O6 K2 106.6(5) . .
W3 O6 K2 100.5(5) . .
W3 O6 W1 120.0(6) . .
W1 O7 K3 101.2(5) . 2_655
W6 O7 K3 108.2(5) . 2_655
W6 O7 W1 149.3(7) . .
W2 O8 K3 105.2(5) . 2_655
W7 O8 K3 107.1(5) . 2_655
W7 O8 W2 145.7(7) . .
W8 O9 W2 152.3(7) . .
W9 O10 W3 151.9(7) . .
W3 O11 K2 106.4(5) . .
W4 O11 K2 104.6(5) . .
W4 O11 W3 147.2(7) . .
W1 O12 K2 103.4(5) . .
W5 O12 K2 102.8(5) . .
W5 O12 W1 151.9(7) . .
W1 O13 Si1 126.5(6) . .
W2 O13 Si1 121.6(6) . .
W2 O13 W1 91.6(4) . .
W3 O13 Si1 124.8(6) . .
W3 O13 W1 92.1(4) . .
W3 O13 W2 90.1(4) . .
W4 O15 K2 101.5(5) . .
W5 O15 K2 108.8(5) . .
W5 O15 W4 120.5(6) . .
K4 O16 Na2 97.1(5) 4_586 .
W5 O16 Na2 163.9(8) . .
W5 O16 K4 97.2(5) . 4_586
W6 O17 W5 153.1(7) . .
W6 O18 K3 137.6(7) . 1_565
W6 O19 K3 102.4(5) . 2_655
W7 O19 K3 103.9(5) . 2_655
W7 O19 W6 120.0(6) . .
K2 O20 Na1 106.3(4) 4_575 .
W7 O20 Na1 147.8(7) . .
W7 O20 K2 104.5(5) . 4_575
W7 O21 K2 94.3(4) . 4_575
W8 O21 K2 97.4(4) . 4_575
W8 O21 W7 154.9(7) . .
W8 O22 K2 106.6(5) . 4_575
W9 O23 W8 116.4(6) . .
W9 O24 K1 163.2(7) . 2_545
W4 O25 K1 100.1(4) . .
W9 O25 K1 103.0(5) . .
W9 O25 W4 154.8(7) . .
W4 O26 Si1 123.5(6) . .
W5 O26 Si1 124.8(6) . .
W5 O26 W4 90.3(4) . .
W11 O26 Si1 124.0(6) . .
W11 O26 W4 93.0(4) . .
W11 O26 W5 91.7(4) . .
W6 O27 Si1 126.0(6) . .
W7 O27 Si1 123.5(6) . .
W7 O27 W6 90.8(4) . .
W10 O27 Si1 122.4(6) . .
W10 O27 W6 92.3(4) . .
W10 O27 W7 92.3(4) . .
W8 O28 Si1 127.0(6) . .
W9 O28 Si1 127.3(6) . .
W9 O28 W8 93.3(4) . .
W4 O29 K1 102.0(5) . .
W11 O29 K1 103.2(4) . .
W11 O29 W4 121.0(6) . .
W5 O30 K4 99.6(5) . 4_586
W11 O30 K4 128.5(5) . 4_586
W11 O30 W5 122.6(6) . .
W10 O31 W6 122.7(6) . .
W10 O32 W7 121.2(6) . .
W8 O33 Gd1 130.5(6) . .
Gd1 O34 K1 97.0(4) . .
W9 O34 K1 104.2(5) . .
W9 O34 Gd1 132.3(6) . .
W10 O35 Gd1 160.8(7) . .
Gd1 O36 K1 98.4(4) . .
W11 O36 K1 104.4(5) . .
W11 O36 Gd1 157.2(6) . .
W11 O37 W10 142.3(7) . .
W11 O38 K1 153.3(6) . 2
W10 O39 K4 137.7(6) . .
Gd1 O40 C2 93.6(10) 3_575 3_575
Gd1 O40 C2 136.6(11) . 3_575
K1 O42 C2 124.0(10) . .
K4 O42 C2 124.2(11) 3_575 .
K4 O42 K1 89.2(4) 3_575 .
Gd1 O42 C2 93.3(10) . .
Gd1 O42 K1 100.7(4) . .
Gd1 O42 K4 126.1(5) . 3_575
K4 O43 K1 93.2(5) 3_575 .
Na2 O47 Na1 97.4(9) . 2_655
K4 O48 Na2 106.9(6) 4_586 .
Na2 O49 Na1 92.3(6) . 2_655
K3 O50 Na2 118.7(7) 4_576 .
O47 Na1 O20 75.9(6) 2_645 .
O49 Na1 O20 148.2(6) 2_645 .
O49 Na1 O47 81.2(7) 2_645 2_645
Na1 Na1 O20 132.6(7) 3_675 .
Na1 Na1 O47 93.3(8) 3_675 2_645
Na1 Na1 O49 69.8(6) 3_675 2_645
O16 Na2 O1 99.4(5) . 3_676
O47 Na2 O1 81.5(7) . 3_676
O47 Na2 O16 90.3(7) . .
O48 Na2 O1 176.8(6) . 3_676
O48 Na2 O16 83.1(5) . .
O48 Na2 O47 100.5(7) . .
O49 Na2 O1 93.7(6) . 3_676
O49 Na2 O16 166.7(6) . .
O49 Na2 O47 89.1(7) . .
O49 Na2 O48 83.9(6) . .
O50 Na2 O1 86.3(6) . 3_676
O50 Na2 O16 94.0(6) . .
O50 Na2 O47 167.6(8) . .
O50 Na2 O48 91.6(6) . .
O50 Na2 O49 89.4(6) . .
O26 Si1 O13 108.2(6) . .
O27 Si1 O13 109.0(6) . .
O27 Si1 O26 107.4(6) . .
O28 Si1 O13 109.2(6) . .
O28 Si1 O26 110.8(6) . .
O28 Si1 O27 112.2(6) . .
O25 K1 O24 126.4(4) . 2
O29 K1 O24 72.9(3) . 2
O29 K1 O25 54.5(3) . .
O34 K1 O24 149.5(4) . 2
O34 K1 O25 53.1(3) . .
O34 K1 O29 93.4(3) . .
O36 K1 O24 92.0(3) . 2
O36 K1 O25 66.3(3) . .
O36 K1 O29 53.6(3) . .
O36 K1 O34 58.7(3) . .
O38 K1 O24 125.2(4) 2_545 2
O38 K1 O25 81.9(3) 2_545 .
O38 K1 O29 123.0(4) 2_545 .
O38 K1 O34 85.2(3) 2_545 .
O38 K1 O36 141.5(4) 2_545 .
O42 K1 O24 98.1(4) . 2
O42 K1 O25 110.2(4) . .
O42 K1 O29 112.8(4) . .
O42 K1 O34 61.6(3) . .
O42 K1 O36 60.7(3) . .
O42 K1 O38 115.9(4) . 2_545
O43 K1 O24 71.6(4) . 2
O43 K1 O25 159.4(4) . .
O43 K1 O29 144.4(4) . .
O43 K1 O34 118.0(4) . .
O43 K1 O36 128.1(4) . .
O43 K1 O38 78.7(4) . 2_545
O43 K1 O42 73.0(4) . .
O53 K1 O24 82.3(4) 4_576 2
O53 K1 O25 83.3(4) 4_576 .
O53 K1 O29 84.6(4) 4_576 .
O53 K1 O34 124.3(4) 4_576 .
O53 K1 O36 137.4(4) 4_576 .
O53 K1 O38 52.5(4) 4_576 2_545
O53 K1 O42 161.9(4) 4_576 .
O53 K1 O43 90.2(4) 4_576 .
O11 K2 O6 55.7(4) . .
O12 K2 O6 53.4(3) . .
O12 K2 O11 65.4(4) . .
O15 K2 O6 92.7(4) . .
O15 K2 O11 55.9(4) . .
O15 K2 O12 53.1(4) . .
O20 K2 O6 74.5(4) 4_576 .
O20 K2 O11 98.4(4) 4_576 .
O20 K2 O12 126.0(4) 4_576 .
O20 K2 O15 153.5(4) 4_576 .
O21 K2 O6 119.2(4) 4_576 .
O21 K2 O11 96.7(4) 4_576 .
O21 K2 O12 162.0(4) 4_576 .
O21 K2 O15 116.0(4) 4_576 .
O21 K2 O20 55.8(3) 4_576 4_576
O22 K2 O6 147.5(4) 4_576 .
O22 K2 O11 92.0(4) 4_576 .
O22 K2 O12 120.1(4) 4_576 .
O22 K2 O15 68.0(3) 4_576 .
O22 K2 O20 111.1(4) 4_576 4_576
O22 K2 O21 55.4(3) 4_576 4_576
O44 K2 O6 93.4(5) . .
O44 K2 O11 146.6(5) . .
O44 K2 O12 86.8(5) . .
O44 K2 O15 121.7(5) . .
O44 K2 O20 82.8(5) . 4_576
O44 K2 O21 110.8(5) . 4_576
O44 K2 O22 118.9(5) . 4_576
O4 K3 O2 133.7(4) 2_645 .
O7 K3 O2 82.8(4) 2_645 .
O7 K3 O4 54.7(4) 2_645 2_645
O8 K3 O2 127.7(4) 2_645 .
O8 K3 O4 53.5(4) 2_645 2_645
O8 K3 O7 64.9(3) 2_645 2_645
O18 K3 O2 144.6(4) 1_545 .
O18 K3 O4 80.0(4) 1_545 2_645
O18 K3 O7 132.6(4) 1_545 2_645
O18 K3 O8 78.0(4) 1_545 2_645
O19 K3 O2 74.6(4) 2_645 .
O19 K3 O4 90.7(4) 2_645 2_645
O19 K3 O7 53.2(3) 2_645 2_645
O19 K3 O8 53.1(3) 2_645 2_645
O19 K3 O18 122.9(4) 2_645 1_545
O45 K3 O2 74.8(5) . .
O45 K3 O4 151.5(5) . 2_645
O45 K3 O7 147.7(5) . 2_645
O45 K3 O8 111.9(5) . 2_645
O45 K3 O18 72.5(5) . 1_545
O45 K3 O19 97.8(5) . 2_645
O50 K3 O2 93.7(5) 4_575 .
O50 K3 O4 80.1(5) 4_575 2_645
O50 K3 O7 102.2(4) 4_575 2_645
O50 K3 O8 131.3(4) 4_575 2_645
O50 K3 O18 80.4(4) 4_575 1_545
O50 K3 O19 153.3(4) 4_575 2_645
O50 K3 O45 102.1(5) 4_575 .
O30 K4 O16 55.1(3) 4_585 4_585
O39 K4 O16 112.6(4) . 4_585
O39 K4 O30 159.7(4) . 4_585
O42 K4 O16 165.9(4) 3_575 4_585
O42 K4 O30 122.4(4) 3_575 4_585
O42 K4 O39 73.6(3) 3_575 .
O43 K4 O16 99.1(4) 3_575 4_585
O43 K4 O30 71.7(4) 3_575 4_585
O43 K4 O39 128.5(4) 3_575 .
O43 K4 O42 68.2(4) 3_575 3_575
O46 K4 O16 110.2(4) . 4_585
O46 K4 O30 76.6(4) . 4_585
O46 K4 O39 95.4(4) . .
O46 K4 O42 81.0(4) . 3_575
O46 K4 O43 110.8(5) . 3_575
O48 K4 O16 64.2(4) 4_585 4_585
O48 K4 O30 105.7(4) 4_585 4_585
O48 K4 O39 78.6(4) 4_585 .
O48 K4 O42 106.3(4) 4_585 3_575
O48 K4 O43 80.5(4) 4_585 3_575
O48 K4 O46 168.5(5) 4_585 .
O51 K4 O16 67.1(4) 1_565 4_585
O51 K4 O30 98.1(4) 1_565 4_585
O51 K4 O39 61.6(4) 1_565 .
O51 K4 O42 125.7(4) 1_565 3_575
O51 K4 O43 166.1(5) 1_565 3_575
O51 K4 O46 74.8(5) 1_565 .
O51 K4 O48 93.8(4) 1_565 4_585
O33 Gd1 C2 160.0(4) . .
O34 Gd1 C2 101.9(4) . .
O34 Gd1 O33 78.1(4) . .
O35 Gd1 C2 115.4(4) . .
O35 Gd1 O33 80.0(4) . .
O35 Gd1 O34 121.9(4) . .
O36 Gd1 C2 73.6(4) . .
O36 Gd1 O33 125.4(4) . .
O36 Gd1 O34 79.2(4) . .
O36 Gd1 O35 71.5(4) . .
O40 Gd1 C2 26.4(4) 3_575 .
O40 Gd1 C2 88.5(4) . .
O40 Gd1 O33 149.9(4) 3_575 .
O40 Gd1 O33 83.8(4) . .
O40 Gd1 O34 128.1(4) 3_575 .
O40 Gd1 O34 153.3(4) . .
O40 Gd1 O35 94.2(4) 3_575 .
O40 Gd1 O35 73.1(4) . .
O40 Gd1 O36 127.6(4) . .
O40 Gd1 O36 79.1(4) 3_575 .
O41 Gd1 C2 81.9(4) . .
O41 Gd1 O33 78.3(4) . .
O41 Gd1 O34 81.6(4) . .
O41 Gd1 O35 143.4(4) . .
O41 Gd1 O36 144.7(4) . .
O41 Gd1 O40 90.1(4) . 3_575
O41 Gd1 O40 75.5(4) . .
O42 Gd1 C2 25.8(4) . .
O42 Gd1 O33 143.6(4) . .
O42 Gd1 O34 76.8(4) . .
O42 Gd1 O35 136.1(4) . .
O42 Gd1 O36 74.6(4) . .
O42 Gd1 O40 108.5(4) . .
O42 Gd1 O40 52.1(4) . 3_575
O42 Gd1 O41 72.3(4) . .
O4 W1 O1 99.9(6) . .
O6 W1 O1 101.0(6) . .
O6 W1 O4 91.6(6) . .
O7 W1 O1 99.6(5) . .
O7 W1 O4 85.9(5) . .
O7 W1 O6 159.3(5) . .
O12 W1 O1 102.7(6) . .
O12 W1 O4 157.1(6) . .
O12 W1 O6 88.1(5) . .
O12 W1 O7 86.4(5) . .
O13 W1 O1 172.0(5) . .
O13 W1 O4 74.2(5) . .
O13 W1 O6 74.0(5) . .
O13 W1 O7 85.6(4) . .
O13 W1 O12 83.7(5) . .
O4 W2 O2 102.1(6) . .
O5 W2 O2 98.6(6) . .
O5 W2 O4 86.4(6) . .
O8 W2 O2 102.4(6) . .
O8 W2 O4 81.9(5) . .
O8 W2 O5 157.6(5) . .
O9 W2 O2 103.9(6) . .
O9 W2 O4 153.8(6) . .
O9 W2 O5 92.2(6) . .
O9 W2 O8 90.1(5) . .
O13 W2 O2 169.6(5) . .
O13 W2 O4 71.1(5) . .
O13 W2 O5 73.4(5) . .
O13 W2 O8 84.8(4) . .
O13 W2 O9 83.4(5) . .
O5 W3 O3 98.2(6) . .
O6 W3 O3 98.1(6) . .
O6 W3 O5 86.4(5) . .
O10 W3 O3 102.9(6) . .
O10 W3 O5 92.3(5) . .
O10 W3 O6 158.9(5) . .
O11 W3 O3 101.8(6) . .
O11 W3 O5 159.3(5) . .
O11 W3 O6 85.9(5) . .
O11 W3 O10 88.1(5) . .
O13 W3 O3 169.6(5) . .
O13 W3 O5 75.1(5) . .
O13 W3 O6 73.8(5) . .
O13 W3 O10 85.5(5) . .
O13 W3 O11 84.4(5) . .
O14 W4 O11 101.3(6) . .
O15 W4 O11 86.5(5) . .
O15 W4 O14 100.5(5) . .
O25 W4 O11 86.8(5) . .
O25 W4 O14 100.1(5) . .
O25 W4 O15 159.2(5) . .
O26 W4 O11 87.0(5) . .
O26 W4 O14 170.6(5) . .
O26 W4 O15 75.7(4) . .
O26 W4 O25 84.3(4) . .
O29 W4 O11 161.2(5) . .
O29 W4 O14 97.4(5) . .
O29 W4 O15 89.5(5) . .
O29 W4 O25 90.6(5) . .
O29 W4 O26 74.2(4) . .
O15 W5 O12 85.6(5) . .
O16 W5 O12 101.5(6) . .
O16 W5 O15 99.9(6) . .
O17 W5 O12 85.0(5) . .
O17 W5 O15 157.0(5) . .
O17 W5 O16 102.6(6) . .
O26 W5 O12 83.5(5) . .
O26 W5 O15 73.4(4) . .
O26 W5 O16 171.4(5) . .
O26 W5 O17 84.7(4) . .
O30 W5 O12 157.5(5) . .
O30 W5 O15 90.3(5) . .
O30 W5 O16 100.9(6) . .
O30 W5 O17 90.4(5) . .
O30 W5 O26 74.1(4) . .
O17 W6 O7 86.6(5) . .
O18 W6 O7 101.3(5) . .
O18 W6 O17 101.0(6) . .
O19 W6 O7 85.2(5) . .
O19 W6 O17 157.7(5) . .
O19 W6 O18 100.9(5) . .
O27 W6 O7 83.7(4) . .
O27 W6 O17 85.0(4) . .
O27 W6 O18 172.3(5) . .
O27 W6 O19 73.5(4) . .
O31 W6 O7 157.1(5) . .
O31 W6 O17 91.5(5) . .
O31 W6 O18 101.4(6) . .
O31 W6 O19 88.0(5) . .
O31 W6 O27 73.5(4) . .
O19 W7 O8 88.0(5) . .
O20 W7 O8 99.0(5) . .
O20 W7 O19 99.9(5) . .
O21 W7 O8 87.7(5) . .
O21 W7 O19 159.1(5) . .
O21 W7 O20 101.0(5) . .
O27 W7 O8 86.9(4) . .
O27 W7 O19 75.7(4) . .
O27 W7 O20 172.6(5) . .
O27 W7 O21 83.7(4) . .
O32 W7 O8 160.8(5) . .
O32 W7 O19 87.6(5) . .
O32 W7 O20 100.2(5) . .
O32 W7 O21 89.8(5) . .
O32 W7 O27 73.9(4) . .
O21 W8 O9 80.9(5) . .
O22 W8 O9 92.0(5) . .
O22 W8 O21 99.6(5) . .
O23 W8 O9 83.6(5) . .
O23 W8 O21 157.5(5) . .
O23 W8 O22 97.2(5) . .
O28 W8 O9 80.6(4) . .
O28 W8 O21 86.6(4) . .
O28 W8 O22 169.5(5) . .
O28 W8 O23 74.7(4) . .
O33 W8 O9 166.8(5) . .
O33 W8 O21 97.6(5) . .
O33 W8 O22 101.2(5) . .
O33 W8 O23 93.8(5) . .
O33 W8 O28 86.3(5) . .
O23 W9 O10 85.5(5) . .
O24 W9 O10 93.9(5) . .
O24 W9 O23 98.5(5) . .
O25 W9 O10 81.2(5) . .
O25 W9 O23 156.1(5) . .
O25 W9 O24 102.1(5) . .
O28 W9 O10 81.5(4) . .
O28 W9 O23 73.9(4) . .
O28 W9 O24 171.3(5) . .
O28 W9 O25 84.5(4) . .
O34 W9 O10 164.3(5) . .
O34 W9 O23 95.4(5) . .
O34 W9 O24 101.5(5) . .
O34 W9 O25 92.3(5) . .
O34 W9 O28 83.6(5) . .
O31 W10 O27 71.5(4) . .
O32 W10 O27 72.6(4) . .
O32 W10 O31 82.2(5) . .
O35 W10 O27 89.1(5) . .
O35 W10 O31 160.5(5) . .
O35 W10 O32 94.3(5) . .
O37 W10 O27 84.1(4) . .
O37 W10 O31 84.1(5) . .
O37 W10 O32 155.7(5) . .
O37 W10 O35 91.9(5) . .
O39 W10 O27 166.2(5) . .
O39 W10 O31 97.0(5) . .
O39 W10 O32 98.9(5) . .
O39 W10 O35 102.6(6) . .
O39 W10 O37 102.6(5) . .
O29 W11 O26 71.8(4) . .
O30 W11 O26 71.6(4) . .
O30 W11 O29 83.1(5) . .
O36 W11 O26 89.9(5) . .
O36 W11 O29 90.9(5) . .
O36 W11 O30 161.5(5) . .
O37 W11 O26 83.5(4) . .
O37 W11 O29 154.9(5) . .
O37 W11 O30 84.7(5) . .
O37 W11 O36 93.8(5) . .
O38 W11 O26 164.8(5) . .
O38 W11 O29 100.4(5) . .
O38 W11 O30 94.8(5) . .
O38 W11 O36 103.5(5) . .
O38 W11 O37 102.4(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 C2 1.52(3) .
C2 O40 1.28(2) 3_575
C2 O42 1.25(2) .
C2 Gd1 2.869(17) .
O1 Na2 2.468(16) 3_676
O1 W1 1.725(13) .
O2 K3 2.785(14) .
O2 W2 1.713(13) .
O3 W3 1.705(13) .
O4 K3 2.814(14) 2_655
O4 W1 1.879(14) .
O4 W2 2.006(14) .
O5 W2 1.912(13) .
O5 W3 1.926(13) .
O6 K2 2.917(13) .
O6 W1 1.915(13) .
O6 W3 1.973(13) .
O7 K3 2.864(12) 2_655
O7 W1 1.947(11) .
O7 W6 1.923(11) .
O8 K3 2.932(13) 2_655
O8 W2 1.945(12) .
O8 W7 1.898(12) .
O9 W2 1.789(12) .
O9 W8 2.089(12) .
O10 W3 1.819(12) .
O10 W9 2.069(12) .
O11 K2 2.779(13) .
O11 W3 1.933(12) .
O11 W4 1.919(13) .
O12 K2 3.005(13) .
O12 W1 1.915(12) .
O12 W5 1.938(13) .
O13 Si1 1.622(12) .
O13 W1 2.356(11) .
O13 W2 2.400(11) .
O13 W3 2.322(11) .
O14 W4 1.707(12) .
O15 K2 2.853(13) .
O15 W4 1.937(12) .
O15 W5 1.922(12) .
O16 Na2 2.383(16) .
O16 K4 3.051(14) 4_586
O16 W5 1.731(13) .
O17 W5 1.915(12) .
O17 W6 1.891(12) .
O18 K3 2.795(13) 1_565
O18 W6 1.718(13) .
O19 K3 3.000(13) 2_655
O19 W6 1.957(12) .
O19 W7 1.922(12) .
O20 Na1 2.730(16) .
O20 K2 2.907(13) 4_575
O20 W7 1.711(12) .
O21 K2 3.060(12) 4_575
O21 W7 1.906(12) .
O21 W8 1.918(12) .
O22 K2 2.937(13) 4_575
O22 W8 1.734(12) .
O23 W8 1.945(11) .
O23 W9 1.933(11) .
O24 K1 2.822(13) 2_545
O24 W9 1.721(12) .
O25 K1 2.990(12) .
O25 W4 1.873(11) .
O25 W9 1.960(11) .
O26 Si1 1.643(11) .
O26 W4 2.309(11) .
O26 W5 2.414(11) .
O26 W11 2.370(11) .
O27 Si1 1.641(11) .
O27 W6 2.394(11) .
O27 W7 2.324(10) .
O27 W10 2.351(11) .
O28 Si1 1.612(12) .
O28 W8 2.244(11) .
O28 W9 2.289(11) .
O29 K1 2.899(12) .
O29 W4 1.922(11) .
O29 W11 1.977(11) .
O30 K4 2.904(12) 4_586
O30 W5 1.845(12) .
O30 W11 2.066(12) .
O31 W6 1.855(11) .
O31 W10 2.042(12) .
O32 W7 1.914(12) .
O32 W10 1.955(11) .
O33 Gd1 2.343(12) .
O33 W8 1.766(12) .
O34 K1 3.078(12) .
O34 Gd1 2.346(11) .
O34 W9 1.798(11) .
O35 Gd1 2.317(12) .
O35 W10 1.757(12) .
O36 K1 3.023(12) .
O36 Gd1 2.349(11) .
O36 W11 1.770(12) .
O37 W10 1.936(11) .
O37 W11 1.903(12) .
O38 K1 2.904(13) 2
O38 W11 1.742(12) .
O39 K4 2.864(12) .
O39 W10 1.730(12) .
O40 Gd1 2.445(11) .
O40 Gd1 2.491(11) 3_575
O41 Gd1 2.400(12) .
O42 K1 2.798(13) .
O42 K4 3.033(13) 3_575
O42 Gd1 2.510(12) .
O43 K1 2.769(17) .
O43 K4 2.871(17) 3_575
O44 K2 2.71(2) .
O45 K3 2.741(18) .
O46 K4 2.716(17) .
O47 Na1 2.59(3) 2_655
O47 Na2 2.40(3) .
O48 Na2 2.302(16) .
O48 K4 2.785(15) 4_586
O49 Na1 2.693(18) 2_655
O49 Na2 2.500(18) .
O50 Na2 2.430(19) .
O50 K3 2.893(18) 4_576
O51 K4 2.751(15) 1_545
O53 K1 3.323(16) 4_575
Na1 Na1 2.23(2) 3_675
